#------------------------------------------------------------------------------
#$Date: 2019-11-23 12:03:07 +0200 (Sat, 23 Nov 2019) $
#$Revision: 233208 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/56/7235658.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7235658
loop_
_publ_author_name
'Saini, Mukesh Kumar'
'Gupta, Rakesh'
'Parbhakar, Swati'
'Kumar Mishra, Anil'
'Mathur, Rashi'
'Hussain, Firasat'
_publ_section_title
;
 Dimeric complexes of rare-earth substituted Keggin-type silicotungstates:
 syntheses, crystal structure and solid state properties
;
_journal_issue                   48
_journal_name_full               'RSC Adv.'
_journal_page_first              25357
_journal_paper_doi               10.1039/C4RA02751E
_journal_volume                  4
_journal_year                    2014
_chemical_formula_moiety         '0.5(C8 Er4 K16 Na8 O208 Si4 W44), 6(O)'
_chemical_formula_sum            'C4 Er2 K8 Na4 O110 Si2 W22'
_chemical_formula_weight         6647.93
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_Int_Tables_number      14
_audit_creation_date             2014-03-26
_audit_creation_method
;
Olex2 1.2
(compiled 2014.03.20 svn.r2914 for OlexSys, GUI svn.r4813)
;
_cell_angle_alpha                90
_cell_angle_beta                 110.788(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   20.0503(6)
_cell_length_b                   12.6340(2)
_cell_length_c                   21.0876(5)
_cell_measurement_reflns_used    26426
_cell_measurement_temperature    149.3
_cell_measurement_theta_max      29.9155
_cell_measurement_theta_min      2.8920
_cell_volume                     4994.1(2)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'olex2.refine (Bourhis et al., 2013)'
_diffrn_ambient_temperature      149.3
_diffrn_detector_area_resol_mean 15.9853
_diffrn_measured_fraction_theta_full 0.9986
_diffrn_measured_fraction_theta_max 0.9986
_diffrn_measurement_device_type  'Xcalibur, Sapphire3'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      -0.0156092000
_diffrn_orient_matrix_UB_12      0.0509051000
_diffrn_orient_matrix_UB_13      -0.0022329000
_diffrn_orient_matrix_UB_21      -0.0343668000
_diffrn_orient_matrix_UB_22      -0.0225468000
_diffrn_orient_matrix_UB_23      -0.0155048000
_diffrn_orient_matrix_UB_31      -0.0026376000
_diffrn_orient_matrix_UB_32      -0.0072796000
_diffrn_orient_matrix_UB_33      0.0323777000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0696
_diffrn_reflns_av_unetI/netI     0.0606
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            75076
_diffrn_reflns_theta_full        26.0218
_diffrn_reflns_theta_max         26.02
_diffrn_reflns_theta_min         2.90
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    27.379
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.14921
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.34.49 (release 20-01-2011 CrysAlis171 .NET)
(compiled Jan 20 2011,15:58:25)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear light pink'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    pink
_exptl_crystal_density_diffrn    4.4207
_exptl_crystal_description       'rect. Prism'
_exptl_crystal_F_000             5767.3014
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.03
_refine_diff_density_max         9.1101
_refine_diff_density_min         -3.7273
_refine_diff_density_rms         0.5802
_refine_ls_d_res_high            0.8100
_refine_ls_d_res_low             7.0260
_refine_ls_goodness_of_fit_ref   1.0307
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     389
_refine_ls_number_reflns         9827
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.0307
_refine_ls_R_factor_all          0.0510
_refine_ls_R_factor_gt           0.0449
_refine_ls_shift/su_max          0.0006
_refine_ls_shift/su_mean         0.0000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0386P)²+316.1018P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1050
_refine_ls_wR_factor_ref         0.1086
_reflns_Friedel_coverage         0.0
_reflns_limit_h_max              23
_reflns_limit_h_min              -24
_reflns_limit_k_max              15
_reflns_limit_k_min              0
_reflns_limit_l_max              26
_reflns_limit_l_min              0
_reflns_number_gt                8822
_reflns_number_total             9827
_reflns_threshold_expression     I>=2u(I)
_cod_data_source_file            c4ra02751e2.cif
_cod_data_source_block           fhms25
_cod_database_code               7235658
_chemical_oxdiff_usercomment     '22 OCT 2013'
_reflns_odcompleteness_completeness 99.81
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
;
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y+1/2,-z+1/2
3 -x,-y,-z
4 x,-y-1/2,z-1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
C1 C -0.1347(10) 1.0824(14) 0.0711(9) 0.021(4) Uiso 1.000000
C2 C -0.0755(8) 1.0103(11) 0.0671(7) 0.009(3) Uiso 1.000000
O1 O 0.4945(6) 0.8715(9) 0.4333(6) 0.021(3) Uiso 1.000000
O2 O 0.4236(6) 0.5761(8) 0.2249(5) 0.016(2) Uiso 1.000000
O3 O 0.2906(6) 0.5636(9) 0.4093(6) 0.019(2) Uiso 1.000000
O4 O 0.4417(6) 0.7488(9) 0.3170(5) 0.018(2) Uiso 1.000000
O5 O 0.3458(6) 0.5977(9) 0.3088(5) 0.018(2) Uiso 1.000000
O6 O 0.3759(6) 0.7412(8) 0.4095(5) 0.016(2) Uiso 1.000000
O7 O 0.4185(6) 0.9546(8) 0.3055(5) 0.011(2) Uiso 1.000000
O8 O 0.3839(5) 0.7892(8) 0.1881(5) 0.009(2) Uiso 1.000000
O9 O 0.2847(6) 0.6471(8) 0.1777(5) 0.014(2) Uiso 1.000000
O10 O 0.2066(6) 0.6363(8) 0.2827(5) 0.012(2) Uiso 1.000000
O11 O 0.2368(6) 0.7733(8) 0.3817(5) 0.014(2) Uiso 1.000000
O12 O 0.3521(6) 0.9463(8) 0.3925(5) 0.014(2) Uiso 1.000000
O13 O 0.3090(5) 0.7944(8) 0.2846(5) 0.009(2) Uiso 1.000000
O14 O 0.1172(6) 0.8437(8) 0.4078(5) 0.016(2) Uiso 1.000000
O15 O 0.2304(6) 0.9753(8) 0.4097(5) 0.014(2) Uiso 1.000000
O16 O 0.3246(6) 1.1461(9) 0.4376(6) 0.018(2) Uiso 1.000000
O17 O 0.3283(6) 1.1027(8) 0.3074(5) 0.014(2) Uiso 1.000000
O18 O 0.4448(6) 1.1638(8) 0.2725(5) 0.014(2) Uiso 1.000000
O19 O 0.4031(6) 0.9965(8) 0.1782(5) 0.012(2) Uiso 1.000000
O20 O 0.3789(6) 0.8687(9) 0.0639(5) 0.018(2) Uiso 1.000000
O21 O 0.2587(6) 0.7992(8) 0.0891(5) 0.013(2) Uiso 1.000000
O22 O 0.2017(6) 0.6020(8) 0.0452(5) 0.015(2) Uiso 1.000000
O23 O 0.1445(5) 0.6106(8) 0.1461(5) 0.009(2) Uiso 1.000000
O24 O 0.0637(6) 0.5815(8) 0.2278(5) 0.012(2) Uiso 1.000000
O25 O 0.1146(5) 0.7840(8) 0.2808(5) 0.009(2) Uiso 1.000000
O26 O 0.2142(5) 0.9450(7) 0.2825(5) 0.0051(19) Uiso 1.000000
O27 O 0.2822(5) 0.9504(7) 0.1943(5) 0.007(2) Uiso 1.000000
O28 O 0.1853(5) 0.7987(7) 0.1842(5) 0.0064(19) Uiso 1.000000
O29 O 0.1025(6) 0.9906(8) 0.3082(5) 0.011(2) Uiso 1.000000
O30 O 0.2033(6) 1.1350(8) 0.3217(5) 0.012(2) Uiso 1.000000
O31 O 0.3088(6) 1.1462(8) 0.1778(5) 0.011(2) Uiso 1.000000
O32 O 0.2768(6) 1.0086(8) 0.0763(5) 0.011(2) Uiso 1.000000
O33 O 0.1141(6) 0.7626(8) 0.0492(5) 0.011(2) Uiso 1.000000
O34 O 0.0430(5) 0.7561(8) 0.1477(5) 0.009(2) Uiso 1.000000
O35 O 0.1461(6) 0.9838(8) 0.0866(5) 0.012(2) Uiso 1.000000
O36 O 0.0752(5) 0.9826(8) 0.1742(5) 0.010(2) Uiso 1.000000
O37 O 0.1837(6) 1.1179(8) 0.1901(5) 0.012(2) Uiso 1.000000
O38 O 0.0664(6) 1.1784(8) 0.2275(5) 0.013(2) Uiso 1.000000
O39 O 0.1864(6) 1.1817(8) 0.0606(5) 0.015(2) Uiso 1.000000
O40 O 0.0329(6) 0.9568(8) -0.0373(5) 0.012(2) Uiso 1.000000
O41 O -0.0414(6) 0.7809(8) -0.0019(5) 0.015(2) Uiso 1.000000
O42 O -0.0681(6) 0.9206(8) 0.0919(5) 0.014(2) Uiso 1.000000
O43 O -0.1742(7) 0.8990(10) 0.1821(6) 0.030(3) Uiso 1.000000
O44 O 0.4577(11) 0.8992(16) 0.5855(10) 0.069(5) Uiso 1.000000
O45 O 0.3934(8) 0.3854(11) 0.3208(7) 0.036(3) Uiso 1.000000
O46 O 0.0774(9) 1.3745(12) -0.0968(8) 0.045(4) Uiso 1.000000
O47 O 0.4675(12) 1.2938(18) 0.4443(11) 0.082(6) Uiso 1.000000
O48 O 0.3161(6) 1.3771(8) 0.4817(5) 0.016(2) Uiso 1.000000
O49 O 0.4715(8) 1.4051(11) 0.5939(7) 0.034(3) Uiso 1.000000
O50 O 0.3675(9) 1.2012(12) 0.6118(8) 0.044(4) Uiso 1.000000
O51 O 0.2268(7) 0.3873(10) 0.0291(6) 0.027(3) Uiso 1.000000
O52 O 0.1640(8) 0.3998(12) 0.1303(7) 0.042(4) Uiso 1.000000
O53 O -0.0302(8) 0.6915(11) -0.1151(7) 0.036(3) Uiso 1.000000
O54 O 0.2561(7) 1.3159(10) 0.2487(6) 0.025(3) Uiso 1.000000
O55 O 0.0496(6) 0.9636(8) 0.4818(5) 0.014(2) Uiso 1.000000
Na1 Na 0.4534(5) 0.9454(7) -0.0119(5) 0.047(2) Uiso 1.000000
Na2 Na 0.4068(5) 1.2564(7) 0.5215(4) 0.0399(19) Uiso 1.000000
Si1 Si 0.2463(2) 0.8711(3) 0.23524(19) 0.0077(8) Uani 1.000000
K1 K -0.02736(18) 0.8826(3) 0.23113(17) 0.0151(7) Uani 1.000000
K2 K 0.3282(2) 0.8430(3) 0.5115(2) 0.0345(11) Uani 1.000000
K3 K 0.4722(2) 0.3683(3) 0.2386(2) 0.0211(8) Uani 1.000000
K4 K 0.1893(3) 1.2369(4) -0.0691(2) 0.0380(11) Uani 1.000000
Er1 Er 0.04520(3) 0.89031(5) 0.07339(3) 0.00783(14) Uani 1.000000
W1 W 0.41388(3) 0.84931(5) 0.36978(3) 0.01141(13) Uani 1.000000
W2 W 0.37049(3) 0.67079(5) 0.24027(3) 0.01143(13) Uani 1.000000
W3 W 0.28838(3) 0.66387(5) 0.35348(3) 0.01156(13) Uani 1.000000
W4 W 0.16179(3) 0.87450(5) 0.35462(3) 0.00912(13) Uani 1.000000
W5 W 0.28478(3) 1.06161(5) 0.37056(3) 0.00961(13) Uani 1.000000
W6 W 0.37698(3) 1.07274(4) 0.24653(3) 0.00826(13) Uani 1.000000
W7 W 0.33781(3) 0.89313(4) 0.12112(3) 0.00896(13) Uani 1.000000
W8 W 0.19215(3) 0.69753(4) 0.09945(3) 0.00849(13) Uani 1.000000
W9 W 0.11129(3) 0.68320(4) 0.21019(3) 0.00823(13) Uani 1.000000
W10 W 0.21511(3) 1.07743(4) 0.11722(3) 0.00787(13) Uani 1.000000
W11 W 0.12451(3) 1.07228(4) 0.23864(3) 0.00813(13) Uani 1.000000
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
_atom_type_scat_dispersion_source
C 0.00347 0.00161 2.31000 1.02000 1.58860 0.86500 20.84390 10.20750 0.56870
51.65120 0.215599998832
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Na 0.03665 0.02467 4.76260 3.17360 1.26740 1.11280 3.28500 8.84220 0.31360
129.42400 0.675999999046
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
K 0.21174 0.26561 8.21860 7.43980 1.05190 0.86590 12.79490 0.77480 213.18700
41.68410 1.42279994488
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
O 0.01158 0.00611 3.04850 2.28680 1.54630 0.86700 13.27710 5.70110 0.32390
32.90890 0.250800013542
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Si 0.08192 0.07060 6.29150 3.03530 1.98910 1.54100 2.43860 32.33370 0.67850
81.69370 1.14069998264
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
W -0.66836 6.76498 29.08180 15.43000 14.43270 5.11982 1.72029 9.22590 0.32170
57.05600 9.88749980927
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
Er -0.12730 5.10226 27.65630 16.42850 14.97790 2.98233 2.07356 0.22354 11.36040
105.70300 5.92046022415
'International Tables Volume C Table 6.1.1.4 (pp. 500-502)'
'Henke, Gullikson and Davis, At. Data and Nucl. Data Tables, 1993, 54, 2'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O40 C2 C1 119.7(13) 3_575 .
O42 C2 C1 120.4(13) . .
O42 C2 O40 119.8(13) . 3_575
Er1 C2 C1 173.1(11) . .
Er1 C2 O40 59.5(7) . 3_575
Er1 C2 O42 60.9(8) . .
W1 O1 Na2 126.7(6) . 3_676
W2 O2 K3 149.4(6) . .
W1 O4 K3 103.6(4) . 2_655
W2 O4 K3 107.0(4) . 2_655
W2 O4 W1 122.1(6) . .
W3 O5 W2 121.3(6) . .
W1 O6 K2 107.1(4) . .
W3 O6 K2 101.6(4) . .
W3 O6 W1 119.9(5) . .
W1 O7 K3 101.4(4) . 2_655
W6 O7 K3 106.8(4) . 2_655
W6 O7 W1 150.4(6) . .
W2 O8 K3 105.9(4) . 2_655
W7 O8 K3 106.5(4) . 2_655
W7 O8 W2 145.7(6) . .
W8 O9 W2 152.0(6) . .
W9 O10 W3 151.8(6) . .
W3 O11 K2 106.5(4) . .
W4 O11 K2 104.6(4) . .
W4 O11 W3 146.9(6) . .
W1 O12 K2 103.8(4) . .
W5 O12 K2 102.9(4) . .
W5 O12 W1 151.8(6) . .
W1 O13 Si1 126.4(5) . .
W2 O13 Si1 121.8(5) . .
W2 O13 W1 92.7(4) . .
W3 O13 Si1 123.4(5) . .
W3 O13 W1 92.4(3) . .
W3 O13 W2 90.7(3) . .
W4 O15 K2 102.5(4) . .
W5 O15 K2 108.1(4) . .
W5 O15 W4 120.5(5) . .
K4 O16 Na2 96.9(4) 4_586 .
W5 O16 Na2 164.7(7) . .
W5 O16 K4 96.7(5) . 4_586
W6 O17 W5 152.6(6) . .
W6 O18 K3 138.3(5) . 1_565
W6 O19 K3 102.9(4) . 2_655
W7 O19 K3 103.9(4) . 2_655
W7 O19 W6 119.5(5) . .
K2 O20 Na1 107.0(4) 4_575 .
W7 O20 Na1 148.2(6) . .
W7 O20 K2 103.9(5) . 4_575
W7 O21 K2 94.3(4) . 4_575
W8 O21 K2 97.7(4) . 4_575
W8 O21 W7 154.5(6) . .
W8 O22 K2 107.7(5) . 4_575
W9 O23 W8 116.1(5) . .
W9 O24 K1 162.1(6) . 2_545
W4 O25 K1 100.1(4) . .
W9 O25 K1 103.9(4) . .
W9 O25 W4 153.9(6) . .
W4 O26 Si1 122.9(5) . .
W5 O26 Si1 124.3(5) . .
W5 O26 W4 90.5(3) . .
W11 O26 Si1 123.9(5) . .
W11 O26 W4 93.4(3) . .
W11 O26 W5 92.5(3) . .
W6 O27 Si1 125.1(5) . .
W7 O27 Si1 124.2(5) . .
W7 O27 W6 91.0(3) . .
W10 O27 Si1 122.1(5) . .
W10 O27 W6 92.5(3) . .
W10 O27 W7 92.6(3) . .
W8 O28 Si1 127.9(5) . .
W9 O28 Si1 127.7(5) . .
W9 O28 W8 93.2(3) . .
W4 O29 K1 101.4(4) . .
W11 O29 K1 103.0(4) . .
W11 O29 W4 121.2(5) . .
W5 O30 K4 98.8(4) . 4_586
W11 O30 K4 128.9(5) . 4_586
W11 O30 W5 122.9(5) . .
W10 O31 W6 122.3(5) . .
W10 O32 W7 121.0(5) . .
W8 O33 Er1 132.4(5) . .
Er1 O34 K1 97.5(3) . .
W9 O34 K1 103.5(4) . .
W9 O34 Er1 133.1(5) . .
W10 O35 Er1 160.7(6) . .
Er1 O36 K1 99.4(3) . .
W11 O36 K1 103.7(4) . .
W11 O36 Er1 156.8(6) . .
W11 O37 W10 142.1(6) . .
W11 O38 K1 151.7(5) . 2
W10 O39 K4 137.2(5) . .
Er1 O40 C2 93.2(8) 3_575 3_575
Er1 O40 C2 136.3(9) . 3_575
K1 O42 C2 123.3(9) . .
K4 O42 C2 124.2(10) 3_575 .
K4 O42 K1 88.4(3) 3_575 .
Er1 O42 C2 93.2(9) . .
Er1 O42 K1 101.4(4) . .
Er1 O42 K4 127.0(4) . 3_575
K4 O43 K1 92.9(4) 3_575 .
Na2 O47 Na1 97.6(8) . 2_655
K4 O48 Na2 107.1(5) 4_586 .
Na2 O49 Na1 92.1(5) . 2_655
K3 O50 Na2 119.1(6) 4_576 .
O47 Na1 O20 76.6(6) 2_645 .
O49 Na1 O20 148.3(5) 2_645 .
O49 Na1 O47 80.8(6) 2_645 2_645
Na1 Na1 O20 132.7(6) 3_675 .
Na1 Na1 O47 91.9(7) 3_675 2_645
Na1 Na1 O49 69.5(5) 3_675 2_645
O16 Na2 O1 98.7(5) . 3_676
O47 Na2 O1 82.0(7) . 3_676
O47 Na2 O16 89.7(7) . .
O48 Na2 O1 178.8(6) . 3_676
O48 Na2 O16 82.4(5) . .
O48 Na2 O47 98.5(7) . .
O49 Na2 O1 94.9(5) . 3_676
O49 Na2 O16 166.1(6) . .
O49 Na2 O47 89.3(7) . .
O49 Na2 O48 84.0(5) . .
O50 Na2 O1 87.0(5) . 3_676
O50 Na2 O16 94.8(5) . .
O50 Na2 O47 168.6(8) . .
O50 Na2 O48 92.5(5) . .
O50 Na2 O49 88.8(5) . .
O26 Si1 O13 109.1(5) . .
O27 Si1 O13 108.3(5) . .
O27 Si1 O26 108.0(5) . .
O28 Si1 O13 108.7(5) . .
O28 Si1 O26 111.1(5) . .
O28 Si1 O27 111.6(5) . .
O25 K1 O24 126.0(3) . 2
O29 K1 O24 71.7(3) . 2
O29 K1 O25 55.4(3) . .
O34 K1 O24 149.0(3) . 2
O34 K1 O25 53.0(3) . .
O34 K1 O29 93.6(3) . .
O36 K1 O24 92.1(3) . 2
O36 K1 O25 66.8(3) . .
O36 K1 O29 54.2(3) . .
O36 K1 O34 58.0(3) . .
O38 K1 O24 124.5(3) 2_545 2
O38 K1 O25 81.2(3) 2_545 .
O38 K1 O29 122.4(3) 2_545 .
O38 K1 O34 86.4(3) 2_545 .
O38 K1 O36 141.8(3) 2_545 .
O42 K1 O24 99.1(3) . 2
O42 K1 O25 109.4(3) . .
O42 K1 O29 112.3(3) . .
O42 K1 O34 60.6(3) . .
O42 K1 O36 59.6(3) . .
O42 K1 O38 117.2(3) . 2_545
O43 K1 O24 72.1(3) . 2
O43 K1 O25 159.2(4) . .
O43 K1 O29 143.8(4) . .
O43 K1 O34 118.1(3) . .
O43 K1 O36 127.5(3) . .
O43 K1 O38 79.3(3) . 2_545
O43 K1 O42 73.6(4) . .
O53 K1 O24 81.9(3) 4_576 2
O53 K1 O25 83.4(3) 4_576 .
O53 K1 O29 84.8(3) 4_576 .
O53 K1 O34 124.9(3) 4_576 .
O53 K1 O36 138.1(3) 4_576 .
O53 K1 O38 51.2(3) 4_576 2_545
O53 K1 O42 162.3(4) 4_576 .
O53 K1 O43 90.1(4) 4_576 .
O11 K2 O6 55.0(3) . .
O12 K2 O6 52.5(3) . .
O12 K2 O11 64.6(3) . .
O15 K2 O6 91.2(3) . .
O15 K2 O11 54.9(3) . .
O15 K2 O12 52.7(3) . .
O20 K2 O6 73.6(3) 4_576 .
O20 K2 O11 95.7(3) 4_576 .
O20 K2 O12 124.9(3) 4_576 .
O20 K2 O15 149.9(4) 4_576 .
O21 K2 O6 117.4(3) 4_576 .
O21 K2 O11 94.2(3) 4_576 .
O21 K2 O12 158.7(3) 4_576 .
O21 K2 O15 114.8(3) 4_576 .
O21 K2 O20 55.2(3) 4_576 4_576
O22 K2 O6 144.1(4) 4_576 .
O22 K2 O11 89.4(3) 4_576 .
O22 K2 O12 120.2(3) 4_576 .
O22 K2 O15 68.0(3) 4_576 .
O22 K2 O20 109.6(3) 4_576 4_576
O22 K2 O21 54.4(3) 4_576 4_576
O44 K2 O6 92.5(5) . .
O44 K2 O11 145.7(5) . .
O44 K2 O12 87.8(5) . .
O44 K2 O15 124.0(5) . .
O44 K2 O20 83.4(5) . 4_576
O44 K2 O21 112.5(5) . 4_576
O44 K2 O22 123.3(5) . 4_576
O4 K3 O2 134.5(3) 2_645 .
O7 K3 O2 83.5(3) 2_645 .
O7 K3 O4 54.9(3) 2_645 2_645
O8 K3 O2 128.4(3) 2_645 .
O8 K3 O4 53.6(3) 2_645 2_645
O8 K3 O7 65.1(3) 2_645 2_645
O18 K3 O2 144.0(3) 1_545 .
O18 K3 O4 79.5(3) 1_545 2_645
O18 K3 O7 132.5(3) 1_545 2_645
O18 K3 O8 78.2(3) 1_545 2_645
O19 K3 O2 74.7(3) 2_645 .
O19 K3 O4 91.5(3) 2_645 2_645
O19 K3 O7 53.7(3) 2_645 2_645
O19 K3 O8 53.7(3) 2_645 2_645
O19 K3 O18 123.7(3) 2_645 1_545
O45 K3 O2 74.4(4) . .
O45 K3 O4 151.1(4) . 2_645
O45 K3 O7 148.3(4) . 2_645
O45 K3 O8 112.1(4) . 2_645
O45 K3 O18 72.5(4) . 1_545
O45 K3 O19 97.9(4) . 2_645
O50 K3 O2 94.5(4) 4_575 .
O50 K3 O4 78.7(4) 4_575 2_645
O50 K3 O7 101.7(4) 4_575 2_645
O50 K3 O8 130.0(4) 4_575 2_645
O50 K3 O18 79.1(4) 4_575 1_545
O50 K3 O19 153.4(4) 4_575 2_645
O50 K3 O45 102.5(4) 4_575 .
O30 K4 O16 55.4(3) 4_585 4_585
O39 K4 O16 113.4(3) . 4_585
O39 K4 O30 159.9(3) . 4_585
O42 K4 O16 166.3(3) 3_575 4_585
O42 K4 O30 122.3(3) 3_575 4_585
O42 K4 O39 72.8(3) 3_575 .
O43 K4 O16 99.1(4) 3_575 4_585
O43 K4 O30 71.7(3) 3_575 4_585
O43 K4 O39 128.4(4) 3_575 .
O43 K4 O42 68.5(3) 3_575 3_575
O46 K4 O16 110.6(4) . 4_585
O46 K4 O30 77.2(4) . 4_585
O46 K4 O39 93.8(4) . .
O46 K4 O42 80.4(4) . 3_575
O46 K4 O43 111.5(4) . 3_575
O48 K4 O16 63.7(3) 4_585 4_585
O48 K4 O30 105.1(3) 4_585 4_585
O48 K4 O39 80.3(3) 4_585 .
O48 K4 O42 107.0(3) 4_585 3_575
O48 K4 O43 79.8(4) 4_585 3_575
O48 K4 O46 168.5(4) 4_585 .
O51 K4 O16 67.9(4) 1_565 4_585
O51 K4 O30 97.8(4) 1_565 4_585
O51 K4 O39 62.1(3) 1_565 .
O51 K4 O42 124.6(4) 1_565 3_575
O51 K4 O43 166.9(4) 1_565 3_575
O51 K4 O46 72.7(4) 1_565 .
O51 K4 O48 95.8(4) 1_565 4_585
O33 Er1 C2 160.4(4) . .
O34 Er1 C2 101.7(4) . .
O34 Er1 O33 78.1(3) . .
O35 Er1 C2 116.0(4) . .
O35 Er1 O33 79.2(4) . .
O35 Er1 O34 121.8(4) . .
O36 Er1 C2 73.2(4) . .
O36 Er1 O33 125.3(4) . .
O36 Er1 O34 79.0(3) . .
O36 Er1 O35 72.3(4) . .
O40 Er1 C2 27.3(4) 3_575 .
O40 Er1 C2 88.6(4) . .
O40 Er1 O33 149.3(3) 3_575 .
O40 Er1 O33 83.8(3) . .
O40 Er1 O34 128.9(3) 3_575 .
O40 Er1 O34 152.7(3) . .
O40 Er1 O35 94.1(4) 3_575 .
O40 Er1 O35 73.6(4) . .
O40 Er1 O36 128.3(3) . .
O40 Er1 O36 79.3(3) 3_575 .
O41 Er1 C2 82.4(4) . .
O41 Er1 O33 78.1(4) . .
O41 Er1 O34 80.7(3) . .
O41 Er1 O35 143.4(4) . .
O41 Er1 O36 144.1(4) . .
O41 Er1 O40 91.0(4) . 3_575
O41 Er1 O40 75.7(4) . .
O42 Er1 C2 25.9(4) . .
O42 Er1 O33 143.6(4) . .
O42 Er1 O34 76.5(3) . .
O42 Er1 O35 136.9(4) . .
O42 Er1 O36 74.3(4) . .
O42 Er1 O40 108.4(3) . .
O42 Er1 O40 53.1(3) . 3_575
O42 Er1 O41 72.3(4) . .
O4 W1 O1 100.1(5) . .
O6 W1 O1 100.8(5) . .
O6 W1 O4 91.4(5) . .
O7 W1 O1 99.7(5) . .
O7 W1 O4 87.2(4) . .
O7 W1 O6 159.3(5) . .
O12 W1 O1 102.3(5) . .
O12 W1 O4 157.4(5) . .
O12 W1 O6 87.3(4) . .
O12 W1 O7 86.1(4) . .
O13 W1 O1 172.0(4) . .
O13 W1 O4 73.9(4) . .
O13 W1 O6 74.5(4) . .
O13 W1 O7 85.3(4) . .
O13 W1 O12 84.1(4) . .
O4 W2 O2 100.6(5) . .
O5 W2 O2 98.7(5) . .
O5 W2 O4 85.9(5) . .
O8 W2 O2 102.2(5) . .
O8 W2 O4 82.8(4) . .
O8 W2 O5 157.8(4) . .
O9 W2 O2 104.2(5) . .
O9 W2 O4 155.1(5) . .
O9 W2 O5 92.2(5) . .
O9 W2 O8 90.0(4) . .
O13 W2 O2 168.7(4) . .
O13 W2 O4 71.2(4) . .
O13 W2 O5 73.3(4) . .
O13 W2 O8 84.9(4) . .
O13 W2 O9 84.4(4) . .
O5 W3 O3 98.1(5) . .
O6 W3 O3 98.8(5) . .
O6 W3 O5 87.1(5) . .
O10 W3 O3 102.6(5) . .
O10 W3 O5 92.1(5) . .
O10 W3 O6 158.5(4) . .
O11 W3 O3 101.7(5) . .
O11 W3 O5 159.7(4) . .
O11 W3 O6 85.5(4) . .
O11 W3 O10 88.0(4) . .
O13 W3 O3 169.0(5) . .
O13 W3 O5 74.5(4) . .
O13 W3 O6 73.0(4) . .
O13 W3 O10 86.1(4) . .
O13 W3 O11 85.3(4) . .
O14 W4 O11 101.1(5) . .
O15 W4 O11 86.8(4) . .
O15 W4 O14 100.6(5) . .
O25 W4 O11 87.2(4) . .
O25 W4 O14 100.2(5) . .
O25 W4 O15 159.1(4) . .
O26 W4 O11 87.7(4) . .
O26 W4 O14 170.2(4) . .
O26 W4 O15 75.4(4) . .
O26 W4 O25 84.4(4) . .
O29 W4 O11 161.1(4) . .
O29 W4 O14 97.7(5) . .
O29 W4 O15 89.0(4) . .
O29 W4 O25 90.2(4) . .
O29 W4 O26 73.4(4) . .
O15 W5 O12 85.6(4) . .
O16 W5 O12 100.9(5) . .
O16 W5 O15 99.7(5) . .
O17 W5 O12 85.3(4) . .
O17 W5 O15 157.6(4) . .
O17 W5 O16 102.1(5) . .
O26 W5 O12 83.8(4) . .
O26 W5 O15 73.5(4) . .
O26 W5 O16 171.4(4) . .
O26 W5 O17 85.2(4) . .
O30 W5 O12 157.1(4) . .
O30 W5 O15 90.0(4) . .
O30 W5 O16 102.0(5) . .
O30 W5 O17 90.4(4) . .
O30 W5 O26 73.4(4) . .
O17 W6 O7 85.8(4) . .
O18 W6 O7 101.6(5) . .
O18 W6 O17 100.9(5) . .
O19 W6 O7 85.8(4) . .
O19 W6 O17 158.5(4) . .
O19 W6 O18 100.2(5) . .
O27 W6 O7 83.6(4) . .
O27 W6 O17 85.7(4) . .
O27 W6 O18 171.8(4) . .
O27 W6 O19 73.7(4) . .
O31 W6 O7 157.1(4) . .
O31 W6 O17 90.9(4) . .
O31 W6 O18 101.2(5) . .
O31 W6 O19 89.2(4) . .
O31 W6 O27 73.6(4) . .
O19 W7 O8 87.8(4) . .
O20 W7 O8 99.8(5) . .
O20 W7 O19 99.9(5) . .
O21 W7 O8 87.5(4) . .
O21 W7 O19 159.3(4) . .
O21 W7 O20 100.7(5) . .
O27 W7 O8 86.8(4) . .
O27 W7 O19 75.8(4) . .
O27 W7 O20 172.1(4) . .
O27 W7 O21 83.9(4) . .
O32 W7 O8 160.3(4) . .
O32 W7 O19 88.0(4) . .
O32 W7 O20 99.9(5) . .
O32 W7 O21 89.7(4) . .
O32 W7 O27 73.6(4) . .
O21 W8 O9 80.5(4) . .
O22 W8 O9 91.9(5) . .
O22 W8 O21 98.5(5) . .
O23 W8 O9 83.5(4) . .
O23 W8 O21 157.6(4) . .
O23 W8 O22 97.6(5) . .
O28 W8 O9 80.4(4) . .
O28 W8 O21 87.2(4) . .
O28 W8 O22 169.7(4) . .
O28 W8 O23 74.8(4) . .
O33 W8 O9 165.7(4) . .
O33 W8 O21 97.2(5) . .
O33 W8 O22 102.3(5) . .
O33 W8 O23 94.5(4) . .
O33 W8 O28 85.4(4) . .
O23 W9 O10 85.6(4) . .
O24 W9 O10 93.7(4) . .
O24 W9 O23 98.7(4) . .
O25 W9 O10 81.3(4) . .
O25 W9 O23 156.7(4) . .
O25 W9 O24 101.3(4) . .
O28 W9 O10 81.5(4) . .
O28 W9 O23 73.8(4) . .
O28 W9 O24 171.3(4) . .
O28 W9 O25 85.2(4) . .
O34 W9 O10 164.0(4) . .
O34 W9 O23 95.3(4) . .
O34 W9 O24 101.9(5) . .
O34 W9 O25 92.1(4) . .
O34 W9 O28 83.5(4) . .
O31 W10 O27 71.6(4) . .
O32 W10 O27 72.7(4) . .
O32 W10 O31 83.1(4) . .
O35 W10 O27 88.7(4) . .
O35 W10 O31 160.0(4) . .
O35 W10 O32 94.4(4) . .
O37 W10 O27 84.1(4) . .
O37 W10 O31 82.9(4) . .
O37 W10 O32 155.7(4) . .
O37 W10 O35 92.0(4) . .
O39 W10 O27 165.6(4) . .
O39 W10 O31 96.6(5) . .
O39 W10 O32 98.2(5) . .
O39 W10 O35 103.4(5) . .
O39 W10 O37 103.0(5) . .
O29 W11 O26 71.9(4) . .
O30 W11 O26 71.2(4) . .
O30 W11 O29 82.8(4) . .
O36 W11 O26 90.3(4) . .
O36 W11 O29 91.4(4) . .
O36 W11 O30 161.5(4) . .
O37 W11 O26 83.3(4) . .
O37 W11 O29 154.7(4) . .
O37 W11 O30 84.5(4) . .
O37 W11 O36 93.7(4) . .
O38 W11 O26 165.2(4) . .
O38 W11 O29 100.8(4) . .
O38 W11 O30 95.4(4) . .
O38 W11 O36 103.0(5) . .
O38 W11 O37 102.1(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 C2 1.52(2) .
C2 O40 1.297(17) 3_575
C2 O42 1.235(17) .
C2 Er1 2.820(15) .
O1 Na2 2.470(15) 3_676
O1 W1 1.717(12) .
O2 K3 2.780(11) .
O2 W2 1.708(11) .
O3 W3 1.719(11) .
O4 K3 2.840(12) 2_655
O4 W1 1.898(11) .
O4 W2 1.997(11) .
O5 W2 1.921(11) .
O5 W3 1.920(11) .
O6 K2 2.941(11) .
O6 W1 1.897(11) .
O6 W3 1.990(11) .
O7 K3 2.881(11) 2_655
O7 W1 1.925(10) .
O7 W6 1.932(10) .
O8 K3 2.924(11) 2_655
O8 W2 1.932(10) .
O8 W7 1.909(10) .
O9 W2 1.783(11) .
O9 W8 2.097(11) .
O10 W3 1.816(10) .
O10 W9 2.066(10) .
O11 K2 2.839(12) .
O11 W3 1.942(10) .
O11 W4 1.901(11) .
O12 K2 3.013(11) .
O12 W1 1.920(10) .
O12 W5 1.927(11) .
O13 Si1 1.635(11) .
O13 W1 2.334(10) .
O13 W2 2.378(10) .
O13 W3 2.330(10) .
O14 W4 1.708(11) .
O15 K2 2.874(11) .
O15 W4 1.931(11) .
O15 W5 1.922(10) .
O16 Na2 2.390(14) .
O16 K4 3.048(12) 4_586
O16 W5 1.725(11) .
O17 W5 1.905(10) .
O17 W6 1.907(10) .
O18 K3 2.786(11) 1_565
O18 W6 1.715(11) .
O19 K3 2.973(11) 2_655
O19 W6 1.952(10) .
O19 W7 1.936(10) .
O20 Na1 2.723(14) .
O20 K2 2.934(12) 4_575
O20 W7 1.713(11) .
O21 K2 3.077(11) 4_575
O21 W7 1.903(10) .
O21 W8 1.919(10) .
O22 K2 2.951(11) 4_575
O22 W8 1.719(10) .
O23 W8 1.938(10) .
O23 W9 1.936(10) .
O24 K1 2.836(11) 2_545
O24 W9 1.717(10) .
O25 K1 2.939(11) .
O25 W4 1.892(10) .
O25 W9 1.942(10) .
O26 Si1 1.654(10) .
O26 W4 2.312(9) .
O26 W5 2.399(9) .
O26 W11 2.343(9) .
O27 Si1 1.646(10) .
O27 W6 2.394(10) .
O27 W7 2.317(9) .
O27 W10 2.339(9) .
O28 Si1 1.600(10) .
O28 W8 2.240(9) .
O28 W9 2.282(9) .
O29 K1 2.877(11) .
O29 W4 1.923(10) .
O29 W11 1.968(10) .
O30 K4 2.909(11) 4_586
O30 W5 1.842(10) .
O30 W11 2.056(10) .
O31 W6 1.850(10) .
O31 W10 2.052(10) .
O32 W7 1.922(10) .
O32 W10 1.946(10) .
O33 Er1 2.296(10) .
O33 W8 1.752(10) .
O34 K1 3.066(10) .
O34 Er1 2.319(9) .
O34 W9 1.784(10) .
O35 Er1 2.273(10) .
O35 W10 1.760(10) .
O36 K1 3.004(10) .
O36 Er1 2.309(10) .
O36 W11 1.776(10) .
O37 W10 1.924(10) .
O37 W11 1.912(10) .
O38 K1 2.917(11) 2
O38 W11 1.737(10) .
O39 K4 2.844(11) .
O39 W10 1.732(10) .
O40 Er1 2.409(10) .
O40 Er1 2.432(10) 3_575
O41 Er1 2.343(11) .
O42 K1 2.796(11) .
O42 K4 3.045(12) 3_575
O42 Er1 2.467(11) .
O43 K1 2.760(14) .
O43 K4 2.864(14) 3_575
O44 K2 2.61(2) .
O45 K3 2.737(14) .
O46 K4 2.732(17) .
O47 Na1 2.57(2) 2_655
O47 Na2 2.40(2) .
O48 Na2 2.291(14) .
O48 K4 2.785(12) 4_586
O49 Na1 2.714(17) 2_655
O49 Na2 2.477(16) .
O50 Na2 2.408(17) .
O50 K3 2.889(16) 4_576
O51 K4 2.713(13) 1_545
O53 K1 3.395(14) 4_575
Na1 Na1 2.233(19) 3_675
